#------------------------------------------------------------------------------
#$Date: 2022-03-24 01:53:55 +0200 (Thu, 24 Mar 2022) $
#$Revision: 273941 $
#$URL: file:///home/coder/svn-repositories/cod/cif/7/70/98/7709810.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7709810
loop_
_publ_author_name
'Wang, Jia'
'Huang, Xiange'
'Li, Hegen'
'Yan, Deyue'
'Huang, Wei'
_publ_section_title
;
 Two Zn(ii) coordination polymers with anticancer drug norcantharidin as
 ligands for cancer chemotherapy
;
_journal_name_full               'Dalton Transactions'
_journal_paper_doi               10.1039/D2DT00300G
_journal_year                    2022
_chemical_formula_moiety         'C96 H96 O72 Zn18.14 [+ solvent]'
_chemical_formula_sum            'C96 H96 O72 Zn18.14'
_chemical_formula_weight         3587.51
_space_group_crystal_system      triclinic
_space_group_IT_number           2
_space_group_name_Hall           '-P 1'
_space_group_name_H-M_alt        'P -1'
_atom_sites_solution_hydrogens   geom
_audit_creation_method           SHELXL-2018/3
_audit_update_record
;
2022-03-03 deposited with the CCDC.	2022-03-09 downloaded from the CCDC.
;
_cell_angle_alpha                107.5880(10)
_cell_angle_beta                 102.592(2)
_cell_angle_gamma                117.1150(10)
_cell_formula_units_Z            1
_cell_length_a                   16.9434(5)
_cell_length_b                   17.4308(5)
_cell_length_c                   17.7700(5)
_cell_measurement_reflns_used    9909
_cell_measurement_temperature    173(2)
_cell_measurement_theta_max      68.36
_cell_measurement_theta_min      4.08
_cell_volume                     4042.7(2)
_computing_structure_refinement  'SHELXL-2018/3 (Sheldrick, 2018)'
_computing_structure_solution    'SHELXT 2018/2 (Sheldrick, 2018)'
_diffrn_ambient_temperature      173(2)
_diffrn_measured_fraction_theta_full 0.998
_diffrn_measured_fraction_theta_max 0.994
_diffrn_measurement_device_type  'Bruker D8 VENTURE'
_diffrn_measurement_method       'φ and ω scans'
_diffrn_radiation_type           CuK\a
_diffrn_radiation_wavelength     1.54178
_diffrn_reflns_av_R_equivalents  0.0539
_diffrn_reflns_av_unetI/netI     0.0402
_diffrn_reflns_Laue_measured_fraction_full 0.998
_diffrn_reflns_Laue_measured_fraction_max 0.994
_diffrn_reflns_limit_h_max       20
_diffrn_reflns_limit_h_min       -20
_diffrn_reflns_limit_k_max       20
_diffrn_reflns_limit_k_min       -21
_diffrn_reflns_limit_l_max       20
_diffrn_reflns_limit_l_min       -21
_diffrn_reflns_number            66758
_diffrn_reflns_point_group_measured_fraction_full 0.998
_diffrn_reflns_point_group_measured_fraction_max 0.994
_diffrn_reflns_theta_full        67.679
_diffrn_reflns_theta_max         68.502
_diffrn_reflns_theta_min         5.131
_exptl_absorpt_coefficient_mu    3.579
_exptl_absorpt_correction_T_max  0.7531
_exptl_absorpt_correction_T_min  0.6366
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
SADABS-2016/2 - Bruker AXS area detector scaling and absorption correction 
;
_exptl_crystal_colour            colourless
_exptl_crystal_density_diffrn    1.474
_exptl_crystal_description       block
_exptl_crystal_F_000             1792
_exptl_crystal_size_max          0.140
_exptl_crystal_size_mid          0.120
_exptl_crystal_size_min          0.100
_refine_diff_density_max         1.468
_refine_diff_density_min         -0.425
_refine_diff_density_rms         0.087
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.064
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     852
_refine_ls_number_reflns         14820
_refine_ls_number_restraints     1
_refine_ls_restrained_S_all      1.064
_refine_ls_R_factor_all          0.0473
_refine_ls_R_factor_gt           0.0388
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0701P)²+2.1385P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1166
_refine_ls_wR_factor_ref         0.1217
_reflns_Friedel_coverage         0.000
_reflns_number_gt                12124
_reflns_number_total             14820
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            d2dt00300g2.cif
_cod_data_source_block           a
_cod_database_code               7709810
_shelx_shelxl_version_number     2018/3
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_shelx_estimated_absorpt_t_min   0.634
_shelx_estimated_absorpt_t_max   0.716
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, -y, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Zn6 Zn 0.60811(4) 0.39367(4) 0.49222(3) 0.0301(2) Uani 0.819(2) 1 d . . . . .
O6 O 0.55062(17) 0.39185(17) 0.37738(15) 0.0322(5) Uani 1 1 d . . . . .
C6 C 0.8565(3) 0.5140(3) 0.3639(3) 0.0449(9) Uani 1 1 d . . . . .
H6 H 0.923284 0.563819 0.373037 0.054 Uiso 1 1 calc R U . . .
Zn7 Zn 0.81056(3) 0.53648(4) 0.64992(3) 0.0365(2) Uani 0.977(2) 1 d . . . . .
O7 O 0.89820(17) 0.81812(18) 0.58287(15) 0.0385(6) Uani 1 1 d . . . . .
C7 C 0.8007(3) 0.5610(3) 0.3809(2) 0.0368(8) Uani 1 1 d . . . . .
Zn8 Zn 0.47360(4) 0.20729(3) 0.50186(3) 0.03466(12) Uani 1 1 d . . . . .
O8 O 0.80536(17) 0.82357(17) 0.65377(14) 0.0347(5) Uani 1 1 d . . . . .
C8 C 0.8150(3) 0.4624(3) 0.4815(3) 0.0397(8) Uani 1 1 d . . . . .
Zn9 Zn 0.55925(3) 0.50601(3) 0.78823(3) 0.02946(11) Uani 1 1 d . . . . .
O9 O 0.68566(17) 0.63074(16) 0.49022(14) 0.0310(5) Uani 1 1 d . . . . .
C9 C 0.8558(3) 0.3999(3) 0.7061(3) 0.0528(11) Uani 1 1 d . . . . .
H9 H 0.849442 0.365200 0.646575 0.063 Uiso 1 1 calc R U . . .
Zn10 Zn 0.40868(5) 0.48259(5) 0.63493(4) 0.0292(3) Uani 0.645(2) 1 d . . . . .
O10 O 0.64748(18) 0.84738(17) 0.61688(15) 0.0355(5) Uani 1 1 d . . . . .
C10 C 0.9299(4) 0.4049(4) 0.7788(4) 0.0695(15) Uani 1 1 d . . . . .
H10A H 0.987467 0.414592 0.767149 0.083 Uiso 1 1 calc R U . . .
H10B H 0.899685 0.345318 0.785991 0.083 Uiso 1 1 calc R U . . .
O11 O 0.7219(2) 0.91270(17) 0.76116(15) 0.0387(6) Uani 1 1 d . . . . .
C11 C 0.9578(4) 0.4943(4) 0.8590(3) 0.0648(13) Uani 1 1 d . . . . .
H11A H 0.942181 0.476981 0.904446 0.078 Uiso 1 1 calc R U . . .
H11B H 1.027993 0.546610 0.884018 0.078 Uiso 1 1 calc R U . . .
O12 O 0.4425(2) 0.79033(19) 0.70710(16) 0.0423(6) Uani 1 1 d . . . . .
C12 C 0.8937(3) 0.5241(3) 0.8203(3) 0.0481(10) Uani 1 1 d . . . . .
H12 H 0.917635 0.593286 0.855829 0.058 Uiso 1 1 calc R U . . .
O13 O 0.44824(19) 0.76118(18) 0.57778(16) 0.0390(6) Uani 1 1 d . . . . .
C13 C 0.7859(3) 0.4504(3) 0.7987(2) 0.0405(9) Uani 1 1 d . . . . .
H13 H 0.781993 0.432343 0.846731 0.049 Uiso 1 1 calc R U . . .
O14 O 0.5522(2) 0.93581(18) 0.55953(17) 0.0438(6) Uani 1 1 d . . . . .
C14 C 0.7245(3) 0.4904(3) 0.7839(2) 0.0351(8) Uani 1 1 d . . . . .
O15 O 0.91625(18) 0.6818(2) 0.71733(17) 0.0427(6) Uani 1 1 d . . . . .
C15 C 0.7583(3) 0.3602(3) 0.7143(3) 0.0445(9) Uani 1 1 d . . . . .
H15 H 0.741570 0.303409 0.726005 0.053 Uiso 1 1 calc R U . . .
O16 O 0.81931(16) 0.72605(16) 0.75143(16) 0.0344(5) Uani 1 1 d . . . . .
C16 C 0.6764(3) 0.3302(3) 0.6322(2) 0.0384(8) Uani 1 1 d . . . . .
O17 O 0.91526(18) 0.93526(17) 0.84251(15) 0.0375(6) Uani 1 1 d . . . . .
C17 C 0.9759(3) 0.9074(3) 0.7384(2) 0.0394(9) Uani 1 1 d . . . . .
H17 H 1.036679 0.938538 0.729224 0.047 Uiso 1 1 calc R U . . .
O18 O 0.73523(17) 0.81020(16) 0.86487(15) 0.0339(5) Uani 1 1 d . . . . .
C18 C 0.9839(3) 0.8524(3) 0.7928(2) 0.0388(9) Uani 1 1 d . . . . .
H18 H 1.047968 0.859268 0.806673 0.047 Uiso 1 1 calc R U . . .
O19 O 0.67438(17) 0.65228(15) 0.81659(14) 0.0308(5) Uani 1 1 d . . . . .
C19 C 0.9823(3) 0.9108(3) 0.8755(2) 0.0413(9) Uani 1 1 d . . . . .
H19 H 0.962116 0.874488 0.909286 0.050 Uiso 1 1 calc R U . . .
O20 O 0.59500(17) 0.57444(16) 0.92754(14) 0.0329(5) Uani 1 1 d . . . . .
C20 C 1.0804(3) 1.0098(3) 0.9297(3) 0.0547(12) Uani 1 1 d . . . . .
H20A H 1.135975 1.003688 0.931324 0.066 Uiso 1 1 calc R U . . .
H20B H 1.088533 1.042089 0.989823 0.066 Uiso 1 1 calc R U . . .
Zn1 Zn 0.62157(3) 0.35132(4) 0.31491(3) 0.03632(12) Uani 1 1 d . . . . .
O1 O 0.73587(19) 0.3476(2) 0.28095(17) 0.0422(6) Uani 1 1 d . . . . .
C1 C 0.8013(3) 0.4300(3) 0.2704(3) 0.0489(10) Uani 1 1 d . . . . .
H1 H 0.767191 0.441938 0.226409 0.059 Uiso 1 1 calc R U . . .
Zn2 Zn 0.78503(3) 0.72396(3) 0.46192(3) 0.03404(12) Uani 1 1 d . . . . .
O2 O 0.86807(19) 0.5163(2) 0.56168(17) 0.0465(7) Uani 1 1 d . . . . .
O21 O 0.47518(17) 0.56747(16) 0.77792(14) 0.0325(5) Uani 1 1 d . . . . .
C21 C 1.0703(3) 1.0649(3) 0.8785(3) 0.0592(13) Uani 1 1 d . . . . .
H21A H 1.070287 1.121060 0.913651 0.071 Uiso 1 1 calc R U . . .
H21B H 1.123336 1.087749 0.858905 0.071 Uiso 1 1 calc R U . . .
O22 O 0.45815(18) 0.69041(17) 0.81145(15) 0.0367(6) Uani 1 1 d . . . . .
C22 C 0.9704(3) 0.9858(3) 0.8009(2) 0.0447(10) Uani 1 1 d . . . . .
H22 H 0.939825 1.012236 0.771482 0.054 Uiso 1 1 calc R U . . .
O23 O 0.64173(16) 0.68980(15) 0.66084(14) 0.0285(5) Uani 1 1 d . . . . .
C23 C 0.9001(2) 0.7448(3) 0.7494(2) 0.0337(8) Uani 1 1 d . . . . .
O24 O 0.53510(16) 0.48428(16) 0.66433(14) 0.0296(5) Uani 1 1 d . . . . .
C24 C 0.8866(2) 0.8446(2) 0.6514(2) 0.0341(8) Uani 1 1 d . . . . .
O25 O 0.33413(17) 0.35970(16) 0.66621(15) 0.0341(5) Uani 1 1 d . . . . .
C25 C 0.6954(2) 0.7322(2) 0.8700(2) 0.0291(7) Uani 1 1 d . . . . .
O26 O 0.45033(17) 0.37472(16) 0.76952(15) 0.0340(5) Uani 1 1 d . . . . .
C26 C 0.6704(3) 0.7342(2) 0.9481(2) 0.0345(8) Uani 1 1 d . . . . .
H26 H 0.710336 0.802386 0.996113 0.041 Uiso 1 1 calc R U . . .
O27 O 0.29141(18) 0.20441(18) 0.51669(16) 0.0363(6) Uani 1 1 d . . . . .
C27 C 0.6884(3) 0.6687(3) 0.9805(2) 0.0368(8) Uani 1 1 d . . . . .
H27 H 0.745798 0.667983 0.975702 0.044 Uiso 1 1 calc R U . . .
O28 O 0.38939(19) 0.16067(18) 0.56496(16) 0.0375(5) Uani 1 1 d . U . . .
C28 C 0.5578(3) 0.6873(2) 0.9266(2) 0.0326(7) Uani 1 1 d . . . . .
H28 H 0.548927 0.735595 0.964458 0.039 Uiso 1 1 calc R U . . .
O29 O 0.14566(18) 0.17175(18) 0.58737(15) 0.0395(6) Uani 1 1 d . . . . .
C29 C 0.5348(3) 0.6059(3) 0.9527(2) 0.0354(8) Uani 1 1 d . . . . .
H29 H 0.463763 0.552594 0.924824 0.043 Uiso 1 1 calc R U . . .
O30 O 0.49030(17) 0.33514(15) 0.52049(15) 0.0303(5) Uani 1 1 d . . . . .
C30 C 0.5807(3) 0.6489(3) 1.0517(2) 0.0473(10) Uani 1 1 d . . . . .
H30A H 0.553944 0.598039 1.070419 0.057 Uiso 1 1 calc R U . . .
H30B H 0.570557 0.699966 1.079877 0.057 Uiso 1 1 calc R U . . .
O31 O 0.59523(19) 0.25523(18) 0.60630(17) 0.0417(6) Uani 1 1 d . . . . .
C31 C 0.6898(3) 0.6919(3) 1.0718(2) 0.0488(11) Uani 1 1 d . . . . .
H31A H 0.730847 0.762831 1.110739 0.059 Uiso 1 1 calc R U . . .
H31B H 0.713558 0.659965 1.098570 0.059 Uiso 1 1 calc R U . . .
O32 O 0.69747(19) 0.38327(18) 0.59472(17) 0.0408(6) Uani 1 1 d . . . . .
C32 C 0.4929(2) 0.6462(2) 0.8310(2) 0.0300(7) Uani 1 1 d . . . . .
O33 O 0.89345(19) 0.5024(2) 0.73392(18) 0.0449(6) Uani 1 1 d . . . . .
C33 C 0.4682(3) 0.8177(3) 0.6532(2) 0.0383(8) Uani 1 1 d . . . . .
O34 O 0.65939(18) 0.47150(18) 0.81231(16) 0.0375(6) Uani 1 1 d . . . . .
C34 C 0.5259(3) 0.9264(3) 0.6804(3) 0.0448(10) Uani 1 1 d . . . . .
H34 H 0.517753 0.961297 0.731005 0.054 Uiso 1 1 calc R U . . .
O35 O 0.74279(18) 0.54001(18) 0.74355(16) 0.0354(5) Uani 1 1 d . . . . .
C35 C 0.4921(4) 0.9453(3) 0.6046(3) 0.0519(11) Uani 1 1 d . . . . .
H35 H 0.420324 0.900079 0.567060 0.062 Uiso 1 1 calc R U . . .
C36 C 0.5304(5) 1.0528(4) 0.6371(3) 0.0722(16) Uani 1 1 d . . . . .
H36A H 0.521374 1.078341 0.690120 0.087 Uiso 1 1 calc R U . . .
H36B H 0.498009 1.063725 0.591867 0.087 Uiso 1 1 calc R U . . .
O36 O 0.69613(16) 0.53621(16) 0.58406(14) 0.0300(5) Uani 1 1 d . . . . .
C37 C 0.6390(5) 1.0988(3) 0.6567(3) 0.0727(17) Uani 1 1 d . . . . .
H37A H 0.657493 1.131037 0.620235 0.087 Uiso 1 1 calc R U . . .
H37B H 0.681026 1.146748 0.718734 0.087 Uiso 1 1 calc R U . . .
C38 C 0.6460(4) 1.0112(3) 0.6334(3) 0.0498(11) Uani 1 1 d . . . . .
H38 H 0.703392 1.021593 0.620038 0.060 Uiso 1 1 calc R U . . .
C39 C 0.6382(3) 0.9748(3) 0.7022(3) 0.0451(10) Uani 1 1 d . . . . .
H39 H 0.678510 1.031137 0.761912 0.054 Uiso 1 1 calc R U . . .
C40 C 0.2673(3) 0.1404(3) 0.6173(2) 0.0373(8) Uani 1 1 d . . . . .
H40 H 0.280164 0.096054 0.634139 0.045 Uiso 1 1 calc R U . . .
C41 C 0.6717(3) 0.9059(2) 0.6925(2) 0.0351(8) Uani 1 1 d . . . . .
C42 C 0.1563(3) 0.0895(3) 0.5664(2) 0.0410(9) Uani 1 1 d . . . . .
H42 H 0.131225 0.048216 0.502668 0.049 Uiso 1 1 calc R U . . .
C43 C 0.1017(3) 0.0363(3) 0.6107(3) 0.0548(12) Uani 1 1 d . . . . .
H43A H 0.127295 -0.000030 0.627111 0.066 Uiso 1 1 calc R U . . .
H43B H 0.030825 -0.009282 0.572900 0.066 Uiso 1 1 calc R U . . .
C44 C 0.1226(3) 0.1202(3) 0.6915(3) 0.0586(13) Uani 1 1 d . . . . .
H44A H 0.061667 0.114886 0.690855 0.070 Uiso 1 1 calc R U . . .
H44B H 0.156579 0.122279 0.745777 0.070 Uiso 1 1 calc R U . . .
C45 C 0.1886(3) 0.2092(3) 0.6820(2) 0.0449(10) Uani 1 1 d . . . . .
H45 H 0.190344 0.268138 0.715101 0.054 Uiso 1 1 calc R U . . .
C46 C 0.2908(3) 0.2276(3) 0.7006(2) 0.0366(8) Uani 1 1 d . . . . .
H46 H 0.314199 0.221319 0.753762 0.044 Uiso 1 1 calc R U . . .
C47 C 0.3635(3) 0.3279(2) 0.7127(2) 0.0328(8) Uani 1 1 d . . . . .
C48 C 0.3212(3) 0.1711(2) 0.5624(2) 0.0331(7) Uani 1 1 d . U . . .
C2 C 0.8692(4) 0.4010(4) 0.2462(4) 0.0678(14) Uani 1 1 d . . . . .
H2A H 0.840372 0.357328 0.183194 0.081 Uiso 1 1 calc R U . . .
H2B H 0.934110 0.458877 0.263021 0.081 Uiso 1 1 calc R U . . .
Zn3 Zn 0.65175(4) 0.71997(4) 0.55820(4) 0.0280(2) Uani 0.736(2) 1 d . . . . .
O3 O 0.72387(18) 0.40843(19) 0.44764(16) 0.0394(6) Uani 1 1 d . . . . .
C3 C 0.8761(4) 0.3481(4) 0.3001(4) 0.0672(14) Uani 1 1 d . . . . .
H3A H 0.850011 0.279457 0.262237 0.081 Uiso 1 1 calc R U . . .
H3B H 0.944375 0.380821 0.341712 0.081 Uiso 1 1 calc R U . . .
Zn4 Zn 0.76188(3) 0.81759(3) 0.75946(3) 0.03077(12) Uani 1 1 d . . . . .
O4 O 0.70907(17) 0.50421(17) 0.34925(16) 0.0369(6) Uani 1 1 d . . . . .
C4 C 0.8126(3) 0.3554(3) 0.3473(3) 0.0503(10) Uani 1 1 d . . . . .
H4 H 0.786980 0.304814 0.367273 0.060 Uiso 1 1 calc R U . . .
Zn5 Zn 0.66853(3) 0.59473(3) 0.68510(3) 0.02757(19) Uani 0.893(2) 1 d . . . . .
O5 O 0.84881(18) 0.65227(19) 0.42461(17) 0.0417(6) Uani 1 1 d . . . . .
C5 C 0.8644(3) 0.4598(3) 0.4192(3) 0.0480(10) Uani 1 1 d . . . . .
H5 H 0.934581 0.486438 0.452148 0.058 Uiso 1 1 calc R U . . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0181 0.0091 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0492 0.0322 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Zn Zn -1.5491 0.6778 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O30 Zn6 O36 104.80(9) . . ?
O30 Zn6 O6 102.96(9) . . ?
O36 Zn6 O6 106.40(9) . . ?
O30 Zn6 O13 80.73(9) . 2_666 ?
O36 Zn6 O13 160.36(10) . 2_666 ?
O6 Zn6 O13 90.30(10) . 2_666 ?
O30 Zn6 O3 161.29(10) . . ?
O36 Zn6 O3 91.23(10) . . ?
O6 Zn6 O3 81.14(9) . . ?
O13 Zn6 O3 81.01(10) 2_666 . ?
O30 Zn6 O32 92.12(10) . . ?
O36 Zn6 O32 80.06(9) . . ?
O6 Zn6 O32 161.14(10) . . ?
O13 Zn6 O32 80.92(10) 2_666 . ?
O3 Zn6 O32 81.02(10) . . ?
O30 Zn6 Zn8 40.35(6) . . ?
O36 Zn6 Zn8 131.43(7) . . ?
O6 Zn6 Zn8 113.14(7) . . ?
O13 Zn6 Zn8 44.49(7) 2_666 . ?
O3 Zn6 Zn8 121.14(7) . . ?
O32 Zn6 Zn8 71.65(7) . . ?
O30 Zn6 Zn1 130.51(7) . . ?
O36 Zn6 Zn1 115.47(7) . . ?
O6 Zn6 Zn1 39.94(7) . . ?
O13 Zn6 Zn1 71.07(7) 2_666 . ?
O3 Zn6 Zn1 44.95(6) . . ?
O32 Zn6 Zn1 121.22(8) . . ?
Zn8 Zn6 Zn1 112.90(2) . . ?
O30 Zn6 Zn7 116.12(7) . . ?
O36 Zn6 Zn7 40.28(7) . . ?
O6 Zn6 Zn7 132.69(7) . . ?
O13 Zn6 Zn7 120.26(7) 2_666 . ?
O3 Zn6 Zn7 70.46(7) . . ?
O32 Zn6 Zn7 44.32(7) . . ?
Zn8 Zn6 Zn7 113.85(2) . . ?
Zn1 Zn6 Zn7 113.16(2) . . ?
Zn1 O6 Zn6 99.40(10) . . ?
Zn1 O6 Zn10 97.43(10) . 2_666 ?
Zn6 O6 Zn10 122.80(12) . 2_666 ?
C7 C6 C1 110.7(3) . . ?
C7 C6 C5 115.1(3) . . ?
C1 C6 C5 101.3(3) . . ?
O36 Zn7 O15 100.89(10) . . ?
O36 Zn7 O2 102.55(10) . . ?
O15 Zn7 O2 92.44(11) . . ?
O36 Zn7 O32 81.35(9) . . ?
O15 Zn7 O32 172.33(11) . . ?
O2 Zn7 O32 94.22(11) . . ?
O36 Zn7 O35 80.23(9) . . ?
O15 Zn7 O35 93.52(10) . . ?
O2 Zn7 O35 172.82(11) . . ?
O32 Zn7 O35 79.58(10) . . ?
O36 Zn7 O33 158.78(10) . . ?
O15 Zn7 O33 92.74(11) . . ?
O2 Zn7 O33 92.93(11) . . ?
O32 Zn7 O33 83.14(10) . . ?
O35 Zn7 O33 82.79(10) . . ?
O36 Zn7 Zn6 40.53(6) . . ?
O15 Zn7 Zn6 139.06(8) . . ?
O2 Zn7 Zn6 86.12(8) . . ?
O32 Zn7 Zn6 45.46(7) . . ?
O35 Zn7 Zn6 91.98(7) . . ?
O33 Zn7 Zn6 128.19(8) . . ?
O36 Zn7 Zn5 40.26(7) . . ?
O15 Zn7 Zn5 85.49(8) . . ?
O2 Zn7 Zn5 140.68(8) . . ?
O32 Zn7 Zn5 91.73(8) . . ?
O35 Zn7 Zn5 44.05(6) . . ?
O33 Zn7 Zn5 126.37(8) . . ?
Zn6 Zn7 Zn5 70.926(17) . . ?
C24 O7 Zn2 123.5(2) . . ?
O4 C7 O5 125.3(4) . . ?
O4 C7 C6 116.4(3) . . ?
O5 C7 C6 118.3(3) . . ?
O30 Zn8 O28 103.03(10) . . ?
O30 Zn8 O31 100.23(10) . . ?
O28 Zn8 O31 89.80(11) . . ?
O30 Zn8 O13 82.06(9) . 2_666 ?
O28 Zn8 O13 173.02(10) . 2_666 ?
O31 Zn8 O13 94.00(11) . 2_666 ?
O30 Zn8 O10 82.15(9) . 2_666 ?
O28 Zn8 O10 95.13(10) . 2_666 ?
O31 Zn8 O10 173.92(11) . 2_666 ?
O13 Zn8 O10 80.74(10) 2_666 2_666 ?
O30 Zn8 O14 161.91(10) . 2_666 ?
O28 Zn8 O14 90.14(10) . 2_666 ?
O31 Zn8 O14 92.05(10) . 2_666 ?
O13 Zn8 O14 83.89(10) 2_666 2_666 ?
O10 Zn8 O14 84.40(10) 2_666 2_666 ?
O30 Zn8 Zn6 40.79(7) . . ?
O28 Zn8 Zn6 140.92(7) . . ?
O31 Zn8 Zn6 85.02(7) . . ?
O13 Zn8 Zn6 45.48(7) 2_666 . ?
O10 Zn8 Zn6 93.33(7) 2_666 . ?
O14 Zn8 Zn6 128.68(8) 2_666 . ?
O30 Zn8 Zn3 41.57(7) . 2_666 ?
O28 Zn8 Zn3 86.93(7) . 2_666 ?
O31 Zn8 Zn3 138.95(8) . 2_666 ?
O13 Zn8 Zn3 94.00(7) 2_666 2_666 ?
O10 Zn8 Zn3 45.20(6) 2_666 2_666 ?
O14 Zn8 Zn3 128.83(8) 2_666 2_666 ?
Zn6 Zn8 Zn3 72.593(18) . 2_666 ?
C24 O8 Zn4 128.7(2) . . ?
C24 O8 Zn3 134.4(2) . . ?
Zn4 O8 Zn3 90.59(9) . . ?
O3 C8 O2 125.3(4) . . ?
O3 C8 C5 116.2(3) . . ?
O2 C8 C5 118.4(3) . . ?
O24 Zn9 O26 102.07(9) . . ?
O24 Zn9 O34 100.06(10) . . ?
O26 Zn9 O34 91.40(10) . . ?
O24 Zn9 O21 83.06(9) . . ?
O26 Zn9 O21 97.11(10) . . ?
O34 Zn9 O21 170.14(10) . . ?
O24 Zn9 O19 81.31(8) . . ?
O26 Zn9 O19 175.67(10) . . ?
O34 Zn9 O19 90.65(10) . . ?
O21 Zn9 O19 80.53(9) . . ?
O24 Zn9 O20 161.83(9) . . ?
O26 Zn9 O20 92.09(9) . . ?
O34 Zn9 O20 90.81(10) . . ?
O21 Zn9 O20 83.94(9) . . ?
O19 Zn9 O20 84.07(8) . . ?
O24 Zn9 Zn10 42.10(7) . . ?
O26 Zn9 Zn10 86.92(7) . . ?
O34 Zn9 Zn10 140.12(8) . . ?
O21 Zn9 Zn10 45.93(6) . . ?
O19 Zn9 Zn10 93.94(6) . . ?
O20 Zn9 Zn10 129.07(7) . . ?
O24 Zn9 Zn5 40.20(6) . . ?
O26 Zn9 Zn5 139.16(7) . . ?
O34 Zn9 Zn5 83.62(7) . . ?
O21 Zn9 Zn5 93.09(7) . . ?
O19 Zn9 Zn5 44.93(6) . . ?
O20 Zn9 Zn5 128.36(6) . . ?
Zn10 Zn9 Zn5 72.374(18) . . ?
Zn2 O9 Zn3 99.43(10) . . ?
Zn2 O9 Zn10 98.89(10) . 2_666 ?
Zn3 O9 Zn10 122.98(12) . 2_666 ?
O33 C9 C15 102.6(3) . . ?
O33 C9 C10 102.3(4) . . ?
C15 C9 C10 109.6(4) . . ?
O6 Zn10 O24 103.98(9) 2_666 . ?
O6 Zn10 O9 105.15(9) 2_666 2_666 ?
O24 Zn10 O9 105.35(9) . 2_666 ?
O6 Zn10 O4 81.38(9) 2_666 2_666 ?
O24 Zn10 O4 160.61(10) . 2_666 ?
O9 Zn10 O4 90.84(10) 2_666 2_666 ?
O6 Zn10 O21 90.51(9) 2_666 . ?
O24 Zn10 O21 80.53(9) . . ?
O9 Zn10 O21 161.02(9) 2_666 . ?
O4 Zn10 O21 80.80(10) 2_666 . ?
O6 Zn10 O25 160.90(10) 2_666 . ?
O24 Zn10 O25 91.87(9) . . ?
O9 Zn10 O25 80.26(9) 2_666 . ?
O4 Zn10 O25 80.22(10) 2_666 . ?
O21 Zn10 O25 81.53(9) . . ?
O6 Zn10 Zn1 40.58(7) 2_666 2_666 ?
O24 Zn10 Zn1 131.10(7) . 2_666 ?
O9 Zn10 Zn1 114.97(7) 2_666 2_666 ?
O4 Zn10 Zn1 44.87(7) 2_666 2_666 ?
O21 Zn10 Zn1 70.41(7) . 2_666 ?
O25 Zn10 Zn1 120.41(7) . 2_666 ?
O6 Zn10 Zn9 114.88(7) 2_666 . ?
O24 Zn10 Zn9 40.97(6) . . ?
O9 Zn10 Zn9 131.85(7) 2_666 . ?
O4 Zn10 Zn9 119.78(7) 2_666 . ?
O21 Zn10 Zn9 44.30(6) . . ?
O25 Zn10 Zn9 70.74(6) . . ?
Zn1 Zn10 Zn9 112.77(2) 2_666 . ?
O6 Zn10 Zn2 132.44(7) 2_666 2_666 ?
O24 Zn10 Zn2 114.81(7) . 2_666 ?
O9 Zn10 Zn2 39.91(6) 2_666 2_666 ?
O4 Zn10 Zn2 71.22(7) 2_666 2_666 ?
O21 Zn10 Zn2 121.16(7) . 2_666 ?
O25 Zn10 Zn2 44.02(6) . 2_666 ?
Zn1 Zn10 Zn2 113.81(3) 2_666 2_666 ?
Zn9 Zn10 Zn2 112.41(2) . 2_666 ?
C41 O10 Zn8 128.7(2) . 2_666 ?
C41 O10 Zn3 135.6(2) . . ?
Zn8 O10 Zn3 90.31(9) 2_666 . ?
C9 C10 C11 101.9(4) . . ?
C41 O11 Zn4 122.3(2) . . ?
C12 C11 C10 101.9(4) . . ?
C33 O12 Zn1 122.5(2) . 2_666 ?
O33 C12 C11 102.3(4) . . ?
O33 C12 C13 102.4(3) . . ?
C11 C12 C13 109.9(4) . . ?
C33 O13 Zn8 127.9(2) . 2_666 ?
C33 O13 Zn6 135.3(2) . 2_666 ?
Zn8 O13 Zn6 90.03(9) 2_666 2_666 ?
C14 C13 C12 111.6(3) . . ?
C14 C13 C15 114.2(3) . . ?
C12 C13 C15 100.9(3) . . ?
C38 O14 C35 96.2(3) . . ?
C38 O14 Zn8 116.4(2) . 2_666 ?
C35 O14 Zn8 117.5(2) . 2_666 ?
O35 C14 O34 125.3(3) . . ?
O35 C14 C13 116.7(3) . . ?
O34 C14 C13 118.1(3) . . ?
C23 O15 Zn7 123.5(2) . . ?
C16 C15 C9 111.3(4) . . ?
C16 C15 C13 114.9(3) . . ?
C9 C15 C13 100.8(3) . . ?
C23 O16 Zn4 128.0(2) . . ?
C23 O16 Zn5 134.8(2) . . ?
Zn4 O16 Zn5 89.95(9) . . ?
O31 C16 O32 125.0(3) . . ?
O31 C16 C15 118.0(3) . . ?
O32 C16 C15 117.0(3) . . ?
C19 O17 C22 95.6(3) . . ?
C19 O17 Zn4 118.4(2) . . ?
C22 O17 Zn4 116.2(2) . . ?
C24 C17 C22 111.0(3) . . ?
C24 C17 C18 114.7(3) . . ?
C22 C17 C18 101.1(3) . . ?
C25 O18 Zn4 122.7(2) . . ?
C19 C18 C23 111.2(3) . . ?
C19 C18 C17 100.9(3) . . ?
C23 C18 C17 114.5(3) . . ?
C25 O19 Zn9 127.8(2) . . ?
C25 O19 Zn5 134.9(2) . . ?
Zn9 O19 Zn5 90.42(8) . . ?
O17 C19 C18 102.6(3) . . ?
O17 C19 C20 103.3(3) . . ?
C18 C19 C20 109.6(3) . . ?
C29 O20 C27 96.7(3) . . ?
C29 O20 Zn9 117.41(19) . . ?
C27 O20 Zn9 115.63(19) . . ?
C19 C20 C21 101.3(3) . . ?
O6 Zn1 O22 102.39(10) . 2_666 ?
O6 Zn1 O12 101.20(10) . 2_666 ?
O22 Zn1 O12 92.01(10) 2_666 2_666 ?
O6 Zn1 O4 82.92(10) . . ?
O22 Zn1 O4 94.28(10) 2_666 . ?
O12 Zn1 O4 171.57(10) 2_666 . ?
O6 Zn1 O1 162.73(10) . . ?
O22 Zn1 O1 90.22(10) 2_666 . ?
O12 Zn1 O1 89.96(11) 2_666 . ?
O4 Zn1 O1 84.42(10) . . ?
O6 Zn1 O3 82.35(10) . . ?
O22 Zn1 O3 172.30(10) 2_666 . ?
O12 Zn1 O3 93.01(10) 2_666 . ?
O4 Zn1 O3 80.18(10) . . ?
O1 Zn1 O3 83.95(10) . . ?
O6 Zn1 Zn10 41.99(7) . 2_666 ?
O22 Zn1 Zn10 86.63(7) 2_666 2_666 ?
O12 Zn1 Zn10 141.13(8) 2_666 2_666 ?
O4 Zn1 Zn10 45.12(7) . 2_666 ?
O1 Zn1 Zn10 128.86(8) . 2_666 ?
O3 Zn1 Zn10 93.10(7) . 2_666 ?
O6 Zn1 Zn6 40.66(7) . . ?
O22 Zn1 Zn6 140.86(8) 2_666 . ?
O12 Zn1 Zn6 85.79(7) 2_666 . ?
O4 Zn1 Zn6 92.83(7) . . ?
O1 Zn1 Zn6 128.79(7) . . ?
O3 Zn1 Zn6 45.53(7) . . ?
Zn10 Zn1 Zn6 71.755(19) 2_666 . ?
C1 O1 C4 96.4(3) . . ?
C1 O1 Zn1 116.6(2) . . ?
C4 O1 Zn1 116.7(2) . . ?
O1 C1 C2 101.3(4) . . ?
O1 C1 C6 102.2(3) . . ?
C2 C1 C6 110.0(4) . . ?
O9 Zn2 O7 100.43(9) . . ?
O9 Zn2 O5 100.80(10) . . ?
O7 Zn2 O5 92.85(11) . . ?
O9 Zn2 O25 83.47(9) . 2_666 ?
O7 Zn2 O25 172.73(10) . 2_666 ?
O5 Zn2 O25 92.43(10) . 2_666 ?
O9 Zn2 O27 81.94(9) . 2_666 ?
O7 Zn2 O27 93.73(10) . 2_666 ?
O5 Zn2 O27 172.30(10) . 2_666 ?
O25 Zn2 O27 80.68(10) 2_666 2_666 ?
O9 Zn2 O29 161.81(10) . 2_666 ?
O7 Zn2 O29 90.56(9) . 2_666 ?
O5 Zn2 O29 93.01(11) . 2_666 ?
O25 Zn2 O29 84.18(9) 2_666 2_666 ?
O27 Zn2 O29 82.93(10) 2_666 2_666 ?
O9 Zn2 Zn3 40.56(7) . . ?
O7 Zn2 Zn3 85.29(7) . . ?
O5 Zn2 Zn3 139.37(8) . . ?
O25 Zn2 Zn3 93.93(7) 2_666 . ?
O27 Zn2 Zn3 45.44(6) 2_666 . ?
O29 Zn2 Zn3 127.55(8) 2_666 . ?
O9 Zn2 Zn10 41.20(7) . 2_666 ?
O7 Zn2 Zn10 139.46(7) . 2_666 ?
O5 Zn2 Zn10 85.00(7) . 2_666 ?
O25 Zn2 Zn10 46.14(6) 2_666 2_666 ?
O27 Zn2 Zn10 92.58(7) 2_666 2_666 ?
O29 Zn2 Zn10 129.96(7) 2_666 2_666 ?
Zn3 Zn2 Zn10 71.262(19) . 2_666 ?
C8 O2 Zn7 121.9(3) . . ?
C32 O21 Zn9 128.7(2) . . ?
C32 O21 Zn10 135.6(2) . . ?
Zn9 O21 Zn10 89.78(9) . . ?
C22 C21 C20 101.8(3) . . ?
C32 O22 Zn1 122.0(2) . 2_666 ?
O17 C22 C17 102.4(3) . . ?
O17 C22 C21 101.4(3) . . ?
C17 C22 C21 111.0(4) . . ?
Zn4 O23 Zn5 99.89(9) . . ?
Zn4 O23 Zn3 98.85(9) . . ?
Zn5 O23 Zn3 124.33(12) . . ?
O15 C23 O16 124.5(3) . . ?
O15 C23 C18 118.8(3) . . ?
O16 C23 C18 116.7(3) . . ?
Zn9 O24 Zn5 100.03(9) . . ?
Zn9 O24 Zn10 96.94(10) . . ?
Zn5 O24 Zn10 125.12(11) . . ?
O7 C24 O8 124.7(3) . . ?
O7 C24 C17 118.5(3) . . ?
O8 C24 C17 116.8(3) . . ?
C47 O25 Zn2 127.6(2) . 2_666 ?
C47 O25 Zn10 134.4(2) . . ?
Zn2 O25 Zn10 89.84(8) 2_666 . ?
O19 C25 O18 125.5(3) . . ?
O19 C25 C26 116.8(3) . . ?
O18 C25 C26 117.7(3) . . ?
C47 O26 Zn9 122.8(2) . . ?
C25 C26 C27 110.8(3) . . ?
C25 C26 C28 114.5(3) . . ?
C27 C26 C28 101.2(3) . . ?
C48 O27 Zn2 128.9(2) . 2_666 ?
C48 O27 Zn3 134.9(2) . 2_666 ?
Zn2 O27 Zn3 89.80(9) 2_666 2_666 ?
O20 C27 C26 102.3(3) . . ?
O20 C27 C31 101.1(3) . . ?
C26 C27 C31 110.1(3) . . ?
C48 O28 Zn8 121.9(2) . . ?
C32 C28 C29 111.0(3) . . ?
C32 C28 C26 114.3(3) . . ?
C29 C28 C26 100.8(3) . . ?
C45 O29 C42 95.7(3) . . ?
C45 O29 Zn2 116.0(2) . 2_666 ?
C42 O29 Zn2 117.2(2) . 2_666 ?
O20 C29 C30 102.5(3) . . ?
O20 C29 C28 102.5(3) . . ?
C30 C29 C28 110.1(3) . . ?
Zn8 O30 Zn6 98.86(10) . . ?
Zn8 O30 Zn3 97.98(9) . 2_666 ?
Zn6 O30 Zn3 125.57(11) . 2_666 ?
C29 C30 C31 101.8(3) . . ?
C16 O31 Zn8 123.9(2) . . ?
C27 C31 C30 101.8(3) . . ?
C16 O32 Zn7 128.9(2) . . ?
C16 O32 Zn6 133.2(2) . . ?
Zn7 O32 Zn6 90.22(9) . . ?
O22 C32 O21 124.4(3) . . ?
O22 C32 C28 118.1(3) . . ?
O21 C32 C28 117.4(3) . . ?
C9 O33 C12 96.1(3) . . ?
C9 O33 Zn7 117.1(2) . . ?
C12 O33 Zn7 116.7(2) . . ?
O13 C33 O12 124.4(3) . . ?
O13 C33 C34 117.3(3) . . ?
O12 C33 C34 118.3(3) . . ?
C14 O34 Zn9 124.3(2) . . ?
C33 C34 C35 110.8(3) . . ?
C33 C34 C39 114.5(3) . . ?
C35 C34 C39 101.6(3) . . ?
C14 O35 Zn5 133.9(2) . . ?
C14 O35 Zn7 129.2(2) . . ?
Zn5 O35 Zn7 90.54(9) . . ?
O14 C35 C36 102.0(4) . . ?
O14 C35 C34 101.7(3) . . ?
C36 C35 C34 110.6(4) . . ?
C35 C36 C37 101.6(4) . . ?
Zn7 O36 Zn6 99.19(10) . . ?
Zn7 O36 Zn5 99.76(10) . . ?
Zn6 O36 Zn5 124.02(11) . . ?
C38 C37 C36 102.4(4) . . ?
O14 C38 C37 101.6(4) . . ?
O14 C38 C39 102.3(3) . . ?
C37 C38 C39 110.7(4) . . ?
C41 C39 C38 110.4(4) . . ?
C41 C39 C34 115.3(3) . . ?
C38 C39 C34 100.5(3) . . ?
C48 C40 C42 110.2(3) . . ?
C48 C40 C46 114.5(3) . . ?
C42 C40 C46 101.2(3) . . ?
O10 C41 O11 125.2(3) . . ?
O10 C41 C39 117.2(3) . . ?
O11 C41 C39 117.6(3) . . ?
O29 C42 C43 102.1(3) . . ?
O29 C42 C40 102.5(3) . . ?
C43 C42 C40 109.4(3) . . ?
C42 C43 C44 102.3(3) . . ?
C45 C44 C43 102.0(3) . . ?
O29 C45 C44 101.4(3) . . ?
O29 C45 C46 102.4(3) . . ?
C44 C45 C46 110.6(4) . . ?
C47 C46 C45 110.9(3) . . ?
C47 C46 C40 114.5(3) . . ?
C45 C46 C40 101.2(3) . . ?
O25 C47 O26 124.0(3) . . ?
O25 C47 C46 118.3(3) . . ?
O26 C47 C46 117.7(3) . . ?
O28 C48 O27 125.2(3) . . ?
O28 C48 C40 117.8(3) . . ?
O27 C48 C40 116.9(3) . . ?
C3 C2 C1 102.1(4) . . ?
O9 Zn3 O23 104.70(9) . . ?
O9 Zn3 O30 105.34(9) . 2_666 ?
O23 Zn3 O30 104.57(9) . 2_666 ?
O9 Zn3 O10 160.80(10) . . ?
O23 Zn3 O10 91.14(9) . . ?
O30 Zn3 O10 80.45(9) 2_666 . ?
O9 Zn3 O8 90.79(10) . . ?
O23 Zn3 O8 80.23(9) . . ?
O30 Zn3 O8 161.04(10) 2_666 . ?
O10 Zn3 O8 81.13(10) . . ?
O9 Zn3 O27 80.80(9) . 2_666 ?
O23 Zn3 O27 160.98(9) . 2_666 ?
O30 Zn3 O27 91.13(9) 2_666 2_666 ?
O10 Zn3 O27 80.80(10) . 2_666 ?
O8 Zn3 O27 81.52(9) . 2_666 ?
O9 Zn3 Zn8 131.69(7) . 2_666 ?
O23 Zn3 Zn8 115.31(7) . 2_666 ?
O30 Zn3 Zn8 40.45(6) 2_666 2_666 ?
O10 Zn3 Zn8 44.48(6) . 2_666 ?
O8 Zn3 Zn8 120.78(7) . 2_666 ?
O27 Zn3 Zn8 70.27(7) 2_666 2_666 ?
O9 Zn3 Zn2 40.02(6) . . ?
O23 Zn3 Zn2 131.68(7) . . ?
O30 Zn3 Zn2 115.05(7) 2_666 . ?
O10 Zn3 Zn2 120.85(7) . . ?
O8 Zn3 Zn2 71.34(7) . . ?
O27 Zn3 Zn2 44.76(7) 2_666 . ?
Zn8 Zn3 Zn2 112.74(2) 2_666 . ?
O9 Zn3 Zn4 114.79(7) . . ?
O23 Zn3 Zn4 40.17(6) . . ?
O30 Zn3 Zn4 131.17(7) 2_666 . ?
O10 Zn3 Zn4 70.86(6) . . ?
O8 Zn3 Zn4 44.34(6) . . ?
O27 Zn3 Zn4 120.90(7) 2_666 . ?
Zn8 Zn3 Zn4 113.19(2) 2_666 . ?
Zn2 Zn3 Zn4 113.52(2) . . ?
C8 O3 Zn1 128.9(2) . . ?
C8 O3 Zn6 135.3(3) . . ?
Zn1 O3 Zn6 89.53(9) . . ?
C4 C3 C2 102.3(4) . . ?
O23 Zn4 O18 101.13(9) . . ?
O23 Zn4 O11 101.96(10) . . ?
O18 Zn4 O11 92.84(10) . . ?
O23 Zn4 O8 81.64(9) . . ?
O18 Zn4 O8 172.69(10) . . ?
O11 Zn4 O8 93.20(10) . . ?
O23 Zn4 O17 160.11(10) . . ?
O18 Zn4 O17 91.51(9) . . ?
O11 Zn4 O17 92.58(10) . . ?
O8 Zn4 O17 84.10(9) . . ?
O23 Zn4 O16 81.02(9) . . ?
O18 Zn4 O16 93.64(10) . . ?
O11 Zn4 O16 172.21(10) . . ?
O8 Zn4 O16 80.05(10) . . ?
O17 Zn4 O16 82.92(9) . . ?
O23 Zn4 Zn3 40.97(6) . . ?
O18 Zn4 Zn3 139.76(7) . . ?
O11 Zn4 Zn3 85.41(7) . . ?
O8 Zn4 Zn3 45.06(6) . . ?
O17 Zn4 Zn3 128.73(7) . . ?
O16 Zn4 Zn3 92.43(7) . . ?
O23 Zn4 Zn5 40.18(6) . . ?
O18 Zn4 Zn5 85.41(7) . . ?
O11 Zn4 Zn5 139.99(8) . . ?
O8 Zn4 Zn5 92.60(7) . . ?
O17 Zn4 Zn5 127.40(7) . . ?
O16 Zn4 Zn5 45.12(6) . . ?
Zn3 Zn4 Zn5 71.320(16) . . ?
C7 O4 Zn1 128.6(2) . . ?
C7 O4 Zn10 135.3(2) . 2_666 ?
Zn1 O4 Zn10 90.01(9) . 2_666 ?
O1 C4 C3 101.4(4) . . ?
O1 C4 C5 102.1(3) . . ?
C3 C4 C5 110.7(4) . . ?
O23 Zn5 O36 104.72(9) . . ?
O23 Zn5 O24 103.99(9) . . ?
O36 Zn5 O24 104.92(9) . . ?
O23 Zn5 O35 160.49(9) . . ?
O36 Zn5 O35 81.25(9) . . ?
O24 Zn5 O35 92.05(9) . . ?
O23 Zn5 O19 90.71(9) . . ?
O36 Zn5 O19 161.45(9) . . ?
O24 Zn5 O19 80.65(8) . . ?
O35 Zn5 O19 80.87(9) . . ?
O23 Zn5 O16 80.64(9) . . ?
O36 Zn5 O16 90.91(9) . . ?
O24 Zn5 O16 161.47(9) . . ?
O35 Zn5 O16 80.71(9) . . ?
O19 Zn5 O16 81.36(9) . . ?
O23 Zn5 Zn7 131.16(7) . . ?
O36 Zn5 Zn7 39.98(6) . . ?
O24 Zn5 Zn7 115.83(7) . . ?
O35 Zn5 Zn7 45.41(7) . . ?
O19 Zn5 Zn7 121.58(7) . . ?
O16 Zn5 Zn7 70.64(7) . . ?
O23 Zn5 Zn4 39.94(6) . . ?
O36 Zn5 Zn4 114.95(6) . . ?
O24 Zn5 Zn4 130.79(7) . . ?
O35 Zn5 Zn4 120.62(7) . . ?
O19 Zn5 Zn4 70.78(6) . . ?
O16 Zn5 Zn4 44.94(7) . . ?
Zn7 Zn5 Zn4 113.219(19) . . ?
O23 Zn5 Zn9 113.51(7) . . ?
O36 Zn5 Zn9 132.28(7) . . ?
O24 Zn5 Zn9 39.77(6) . . ?
O35 Zn5 Zn9 72.27(7) . . ?
O19 Zn5 Zn9 44.65(6) . . ?
O16 Zn5 Zn9 121.82(7) . . ?
Zn7 Zn5 Zn9 115.133(19) . . ?
Zn4 Zn5 Zn9 112.661(19) . . ?
C7 O5 Zn2 122.5(2) . . ?
C8 C5 C4 110.8(4) . . ?
C8 C5 C6 114.9(3) . . ?
C4 C5 C6 101.4(3) . . ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Zn6 O30 2.042(2) . ?
Zn6 O36 2.042(2) . ?
Zn6 O6 2.045(2) . ?
Zn6 O13 2.202(3) 2_666 ?
Zn6 O3 2.209(3) . ?
Zn6 O32 2.211(3) . ?
Zn6 Zn8 3.0878(7) . ?
Zn6 Zn1 3.0960(7) . ?
Zn6 Zn7 3.1025(7) . ?
O6 Zn1 2.015(2) . ?
O6 Zn10 2.072(2) 2_666 ?
C6 C7 1.529(6) . ?
C6 C1 1.544(6) . ?
C6 C5 1.580(6) . ?
Zn7 O36 2.032(2) . ?
Zn7 O15 2.038(3) . ?
Zn7 O2 2.044(3) . ?
Zn7 O32 2.168(3) . ?
Zn7 O35 2.220(3) . ?
Zn7 O33 2.222(3) . ?
Zn7 Zn5 3.1165(7) . ?
O7 C24 1.258(4) . ?
O7 Zn2 2.048(2) . ?
C7 O4 1.260(4) . ?
C7 O5 1.263(5) . ?
Zn8 O30 2.023(2) . ?
Zn8 O28 2.036(3) . ?
Zn8 O31 2.053(3) . ?
Zn8 O13 2.164(3) 2_666 ?
Zn8 O10 2.164(2) 2_666 ?
Zn8 O14 2.181(3) 2_666 ?
Zn8 Zn3 3.0889(8) 2_666 ?
O8 C24 1.267(4) . ?
O8 Zn4 2.175(2) . ?
O8 Zn3 2.203(2) . ?
C8 O3 1.249(4) . ?
C8 O2 1.259(5) . ?
C8 C5 1.528(6) . ?
Zn9 O24 2.030(2) . ?
Zn9 O26 2.044(2) . ?
Zn9 O34 2.048(3) . ?
Zn9 O21 2.146(2) . ?
Zn9 O19 2.196(2) . ?
Zn9 O20 2.196(2) . ?
Zn9 Zn10 3.0731(8) . ?
Zn9 Zn5 3.1242(6) . ?
O9 Zn2 2.024(2) . ?
O9 Zn3 2.047(2) . ?
O9 Zn10 2.078(2) 2_666 ?
C9 O33 1.460(5) . ?
C9 C15 1.534(6) . ?
C9 C10 1.542(6) . ?
Zn10 O24 2.075(2) . ?
Zn10 O4 2.176(3) 2_666 ?
Zn10 O21 2.208(2) . ?
Zn10 O25 2.248(2) . ?
Zn10 Zn1 3.0710(9) 2_666 ?
Zn10 Zn2 3.1173(8) 2_666 ?
O10 C41 1.250(4) . ?
O10 Zn3 2.192(2) . ?
C10 C11 1.542(8) . ?
O11 C41 1.262(4) . ?
O11 Zn4 2.052(3) . ?
C11 C12 1.526(6) . ?
O12 C33 1.266(5) . ?
O12 Zn1 2.053(3) 2_666 ?
C12 O33 1.464(5) . ?
C12 C13 1.546(6) . ?
O13 C33 1.258(4) . ?
C13 C14 1.514(5) . ?
C13 C15 1.593(6) . ?
O14 C38 1.456(5) . ?
O14 C35 1.461(5) . ?
C14 O35 1.259(4) . ?
C14 O34 1.262(5) . ?
O15 C23 1.252(5) . ?
C15 C16 1.523(5) . ?
O16 C23 1.266(4) . ?
O16 Zn4 2.203(3) . ?
O16 Zn5 2.209(2) . ?
C16 O31 1.238(5) . ?
C16 O32 1.266(4) . ?
O17 C19 1.455(5) . ?
O17 C22 1.462(4) . ?
O17 Zn4 2.186(2) . ?
C17 C24 1.525(5) . ?
C17 C22 1.533(6) . ?
C17 C18 1.579(5) . ?
O18 C25 1.256(4) . ?
O18 Zn4 2.047(2) . ?
C18 C19 1.529(5) . ?
C18 C23 1.533(5) . ?
O19 C25 1.253(4) . ?
O19 Zn5 2.206(2) . ?
C19 C20 1.533(5) . ?
O20 C29 1.450(5) . ?
O20 C27 1.461(4) . ?
C20 C21 1.545(7) . ?
Zn1 O22 2.047(2) 2_666 ?
Zn1 O4 2.167(2) . ?
Zn1 O1 2.172(3) . ?
Zn1 O3 2.187(2) . ?
O1 C1 1.459(5) . ?
O1 C4 1.474(5) . ?
C1 C2 1.542(6) . ?
Zn2 O5 2.052(3) . ?
Zn2 O25 2.166(2) 2_666 ?
Zn2 O27 2.187(3) 2_666 ?
Zn2 O29 2.217(2) 2_666 ?
Zn2 Zn3 3.1057(8) . ?
O21 C32 1.257(4) . ?
C21 C22 1.541(5) . ?
O22 C32 1.244(4) . ?
O23 Zn4 2.032(2) . ?
O23 Zn5 2.042(2) . ?
O23 Zn3 2.065(2) . ?
O24 Zn5 2.048(2) . ?
O25 C47 1.259(4) . ?
C25 C26 1.531(5) . ?
O26 C47 1.269(4) . ?
C26 C27 1.538(5) . ?
C26 C28 1.590(5) . ?
O27 C48 1.276(4) . ?
O27 Zn3 2.213(2) 2_666 ?
C27 C31 1.541(5) . ?
O28 C48 1.243(5) . ?
C28 C32 1.529(5) . ?
C28 C29 1.533(5) . ?
O29 C45 1.467(4) . ?
O29 C42 1.473(5) . ?
C29 C30 1.528(5) . ?
O30 Zn3 2.070(2) 2_666 ?
C30 C31 1.547(6) . ?
C33 C34 1.527(5) . ?
C34 C35 1.534(5) . ?
C34 C39 1.580(6) . ?
O35 Zn5 2.167(2) . ?
C35 C36 1.530(6) . ?
C36 C37 1.535(9) . ?
O36 Zn5 2.044(2) . ?
C37 C38 1.524(6) . ?
C38 C39 1.543(5) . ?
C39 C41 1.528(5) . ?
C40 C48 1.525(5) . ?
C40 C42 1.547(5) . ?
C40 C46 1.579(5) . ?
C42 C43 1.521(5) . ?
C43 C44 1.538(7) . ?
C44 C45 1.532(5) . ?
C45 C46 1.546(6) . ?
C46 C47 1.522(5) . ?
C2 C3 1.537(8) . ?
Zn3 Zn4 3.1123(7) . ?
C3 C4 1.528(6) . ?
Zn4 Zn5 3.1183(6) . ?
C4 C5 1.537(6) . ?
